Gel Permeation Chromatography : Band-Broadening and Title...
Embed Size (px)
Transcript of Gel Permeation Chromatography : Band-Broadening and Title...
TitleGel Permeation Chromatography : Band-Broadening andSkewing in High Speed Ge Permeation Chromatography(Special Issue on Polymer Chemistry XII)
Author(s) Kotaka, Tadao; Suzuki, Hidematsu; Inagaki, Hiroshi
Citation Bulletin of the Institute for Chemical Research, KyotoUniversity (1976), 54(2): 100-111
Issue Date 1976-07-20
Type Departmental Bulletin Paper
Bull. Inst. Chem. Res.; Kyoto Univ., Vol. 54, No. 2, 1976
Gel Permeation Chromatography: Band-Broadening
and Skewing in High Speed Gel Permeation
Tadao KOTAKA, Hidematsu SUZUKI, and Hiroshi INAGAKI*
Received March 31, 1976
A computer simulation of gel permeation chromatographic (GPC) fractionation of polymers was carried out with introducing a simple skewed function as the band-spreading function. With the aid of these results as well as those of actual GPC experiments on narrow distribution polystyrenes, a
phenomenological method was proposed for calibrating a GPC unit for band-broadening and skewing phenomena, which one often encounters on operating a high speed GPC. The performance of a high
speed GPC was discussed in regard with such phenomena.
Gel permeation chromatography') (GPC) is now a most routinely used method of determining molecular weight distribution (MWD) of polymers. One of the two recent progresses in this area was the development of GPC gels with small particle size, which led to so-called high speed GPC.2-'4) The other was the installation of molecular weight (MW) detecter which enabled one to monitor MWs of GPC ef-fluents in a continuous fashion.5.6) However, even in such GPC units the basic separation mechanism is the same as in any other conventional GPC units : Resulting chromatograms are subject to the dispersion or band-broadening effects due to imper-fect resolution of GPC columns.7-'9) In a previous article)) we discussed the
dispersion effects on MW-monitor-installed GPC unit on the basis of Tung's phe-nomenological scheme,7, 8) which assumes that a pure compound gives a Gaussian shape chromatogram with the dispersion depending on various factors of a GPC unit employed and on its operating conditions?-4,12)
In this study we have examined the effects on high speed GPC in some detail. With such a GPC one often encounters even for pure compounds skewed chromatograms that show significant tailing toward large elution volume side. Accordingly upon making the dispersion correction, Tung's scheme should be modified to take account of band tailing. Here we will discuss this problem. However, we do not intend either to explore the mechanisms of such phenomena or to examine the effects of operating conditions on the extent of dispersion phenomena. We confine ourselves to a phe-nomenological analysis to establish an adequate method of calibrating GPC unit for such band-broadening and skewing phenomena. Specifically we assume a simple dispersion-correction function, and carry out a computer simulation of the fractionation
* /1NA , to j : Laboratory of Polymer Separation and Characterization, Insti- tute for Chemical Research, Kyoto University, Uji, Kyoto 611.
High Speed GPC
process. These results will be compared with the performance of an actual high speed GPC as well as of a conventional GPC available to us.
Computer Simulation Method The procedures of the simulation are the same as those in our preceding two
papers,'°' 11) except here we use a skewed correction function instead of a symmetrical Gaussian function employed previously by Tung.7.8) We assume a log M versus elution volume v (or y) calibration with a permeability limit vL as
v=f (log M)(1)
Using Eq. (1), we hypothetically fractionate a sample with a normalized MWD function w(log M) to construct a chromatogram F(yt)oy, which should be the hy-pothetical chromatogram obtained if the GPC unit has unlimited resolution but the permeability limit yL :
F(yi ,)8y=Ew (log M;)B log M (y
T. KOTAKA, H. SuzuKI, and H. INAGAKI
1.0• ° ~• h 0.5
° h =3 .0
h h =2.0
pd = 0.5•
-2-1 01 23 ELUTION VOLUME DIFFERENCE (V - Ve)/ml
Fig. 1. Properties of Tung's Gaussian spreading function Eq. 4 (above) and present skewed function Eq. 5 (below). Symbols are the chro-
matograms of standard polystyrenes 11 (0), 4b (4), and 14b (A) obtained on the high-speed GPC with 4 ml/min flow-rate.
Eq. (4) or with Eq. (5), we can calculate various GPC average MWs, which we call apparent averages,11,12) and denote the number average by M:PP, the weight average
by M:,243, etc. On carrying out the simulation we need to have two calibrations, i.e., log M
and a versus v calibration (or h versus v for the symmetric correction case). For a high speed GPC, both of these are somewhat problematic, as we will come back to these problems later. To establish a method of calibration, we first assume at(=a)
be independent of v, and assume the log M versus v calibration as determined by the conventional elution standard method be valid also. For certain model cases, we further assume two simple two-parameter MWD functions, i.e., the log-normal distribution:
w(M)d log M=(2.3026/(3n)112 exp [—(1/82)ln2(M/Mo)]d log M (6a)
Mn = M0 exp (— 82/4)(6b)
Mu, = Mo exp (j92/4)(6c)
Ma,/Mu = Y= exp (82/2)(6d)
and the Schulz distribution:
w(M) log M=[2.30262a+1/T(a+1)]Ma+l exp (-2M)d log M (7a)
High Speed GPC
Y=1 + 1/a(7c)
We examined the shape of G(v) of such model polymers, assuming adequate a values and the log M versus v relation. Analysis of true and apparent MWs from w(M) and G(v), respectively, provides criteria for establishing the calibration for band-broadening and skewing of a GPC unit.
Gel Permeation Chromatographic Experiments A Waters high speed GPC model ALC/GPC 202/R401 (Water Associates, Milford,
Mass.) was employed. Four columns (each 7 mm inner diameter and 30 cm length) of p-styragel® of 106, 106, 104, and 103 A nominal pore size were used. The carrier solvent was THF, and the flow-rates were 1, 2, and 4 ml/min. At the highest rate only 13 minutes were necessary to complete a run. The total numbers of theoretical plates as determined by acetone were 8,291, 8.395, and 10,936, respectively. The injections were usually 0.3 ml of 0.03 to 0.25% stock solutions. Table I summarizes elution data of standard narrow distribution polystyrenes at the three different rates.
Table I. Peak Elution Volume Data of Narrow Distribution Polystyrene on High Speed GPC Unit
Polystyrene Samples*Peak Elution Volume ve (ml)
Code10-4 M„,Y=MwM„Flow rate (ml/min) 4 21
BENZENE0.00781.0047.0 46.7 46.1 11b0.401.0639.4 39.1 38.6
8b1.001.0436.7 36.7 36.1 7b3.70
T. KOTAKA, H. SUZUKI, and H. INAGAKI
RESULTS AND DISCUSSION
Evaluation of Skewness Parameter
First we consider a simulation of model GPC experiments to elucidate a method of determining skewness parameter a as a function of elution volumes. To do this first we need to have log M versus v calibration. For a conventional GPC unit this is usually done with narrow distribution standards by plotting their log (nominal weight average value M,,,) against peak elution volume ve. However, a high speed GPC often gives skewed chromatograms even for narrow distribution standards. Therefore, the above procedure might not be legitimate, because the elution-peak MWs might differ greatly from the true MWs of the standard polystyrenes in such skewed chromatograms unless the standards are indeed monodisperse. The extent of such discrepancy is expected to depend on the extent of band broadening and skewing. The two calibrations are closely related with each other: To determine the log M versus v calibration, we need to know the a versus v calibration and vice versa.
As a working hypothesis we first assumed the MW calibration be given by an adequately drawn smooth curve of log M,u versus ve plots such as those listed in Table I. Figure 2 shows such a curve for 4 ml/min run. Then using this calibration,
~II^ N 5 >a-
ELUTION VOLUME V/mi
Fig. 2. Logarithmic (molecular weight) versus elution volume calibra- tions for 4 ml/min flow-rate runs: Solid curve is from log M.u, versus
ve plots (0), and broken curve from log M, versus v, plots after first iterative simulation (A for Schulz MWD and A for log-normal
MWD and Schulz MWD, wherever they coincide with each other).
High Speed GPC
t:,,/ 101 = 0.8 ±- 8 1 10
2.0 -- 7
x o —\
w0(= 1.2 fao
1.5 —— 5
kl/Wirikat>> Cab), iiiiii634011111h6.01 = 3.0
1.0 ., o > ) ) ) ~ > ) ) ) `) ) ) > > 7 - 3
I I I 253035 4045
ELUTION VOLUME V/m1 Fig. 3. Plots of Y/YdPP values against peak elution volume ve from simu-
lated chromatograms of Schulz type (0) and log-normal type (e) model polymers of narrow distributions (Y=1.04— 1.15), and of
hypothetical monodisperse polymers (Y=1.00: solid curves), using log M4 versus ve calibration and given constant a values as indicated.
Half-lines are from experimental chromatograms of standard polysty- renes: Lower ends indicate the values with nominal Y values, and
upper ends those with Y=1.00.
we calculated various apparent MWs from observed chromatograms of the standard
polystyrenes on one hand, and carried out a simulation on model polymers, on the other, with assuming several different a values. Figure 3 shows examples of YaPP/Y versus ve plots from both simulated and actual GPC experiments. Comparing these two results, we could assign a values and simultaneously estimate peak MW values Me adequate to the standard polystyrenes. These Me versus ve data were used to reconstruct the MW calibration, which is also shown in Fig. 2.
We repeated the above procedures until the calibrations and various average MWs of simulated and actual GPC experiments consistently come to agreement before and after the procedure. To achieve this, only one or two iterations were
T. KOTAKA, H. SUZUKI, and H. INAGAEI
sufficient: In fact the original log Mu, versus ve curve was already a good approxima-tion. The shift of only as much as 0.02 logarithmic unit was necessary to obtain the first log Me versus ve calibration (see Fig. 2), which was good enough to be employed as the MW calibration. With this calibration, various apparent MWs from experi-mental and simulated chromatograms were calculated and found to be in satisfactory agreement with each other. These MW values calculated during the second iteration could be used to reassign a versus ve relation (which did not differ from the first one) .
By this way we could establish both the log Me and a versus ve relations for the high speed GPC unit for calibrating band broadening and skewing. Figure 4
(ii) 1.0 -—
(iii) 0.5 --
253035 40 ELUTION VOLUME V/m1
Fig. 4. Plots of a versus v relations estimated from the data such as given in Fig. 3. Lines indicate possible choices of a versus v relations.
See Eqs. 8a-c.
shows the a versus ve relation, for which several choices are possible, because of the ambiguities of experimental data such as nominal Mu, values of the standard polysty-renes, base-line instability of chromatograms, etc. Although they are rather arbitrary, the choices are:
(i) Sloppy choice:
a = 2.00 for all v(8a)
(ii) Optimistic choice:
a=2.718 for v>29.0
a=exp(0.2632v-6.632) for v
High Speed GPO•
(iii) Pessimistic choice:
a=2.00 for v>>>34.0
a = exp (0.1115v —3.0983) for v
T. KOTAKA, H. SUZUKI, and H. INAGAKI
I I I I I I I
1.4 --\e—— 7 –\--e—1.2
O. O.4 O
1.1 —O~O44 >—4•
. 1.0——3— o 4,—1.0
I I I I I I I I 25 30 3540 45 25 30 3540 45
ELUTION VOLUME V/ml Fig. 5. The performance of the high speed GPC unit (4 ml/min flow rate) as demonstrated
by the plots of YaaP/Y (left) and MVP IM,, (right) from simulated chromatograms of Schulz type (open marks) and log-normal type (closed marks) model polymers of nar-
row (Y=1.05: circles) and broad (Y=2.00: squares) distributions. Solid curves are for hypothetical pure compounds (Y=1.00). The simulations were carried out using
the first log M, versus v, calibration and the Eq. 8b a versus v, relation.
straight line MW calibration in the elution volume range as wide as possible. Even for a GPC unit which has a distorted MW calibration, the Yd1 P/Y versus
v, plots of narrow MWD samples (perhaps Y
High Speed GPC
thetical chromatogram F (v) such as defined by Eq. (2). The F (v) is entirely different from the true MWD, when the sample contains a substantial amount of high MW
components that exceed the vL limit.ii) The deconvolution usually demands the full and accurate knowledges of the experimental chromatogram, which are often
very difficult to achieve in actual experiments. In that sense a computer simulation experiment, which always provides such knowledges, does not necessarily guarantee the performance of any deconvolution methods when being applied to an actual
chromatogram. Because of these reasons, it may not be worthwhile to carry out a tedious deconvolution process to deduce the true MWD. Here we employ a very
simple method of evaluating the band-skewing correction: That is, we use the YaVVI Y, M z"9/Mw, etc. values simulated on certain simple model polymers using the log M
and a calibrations established as above. Table III summarizes the results for a
Table III. Apparent and Corrected MW Data of Two Broad Distribution Polystyrenes Obtained on High Speed GPC (Flow Rate=4 ml/min)
High SpeedCorrected Values Assuming GPC ApparentSCHULZ LOG NORMAL
RAPRA PS 2 (10-4 M,,,=33.3)* ve(28.06) 10-4 M,,,11.3913.40 13.72 10-4 Mw29.6730.61 29.37 Y2.612.284 2.144
NBS 706 (10-4 M,i=12.28: 10-4Mw=25.78: Y=2.10)** ve (28.40) 10-4 M.11.0512.7412.97 10-4 M,„25.8226.9325.97 Y2.342.1142.00.8 * Rubber and Plastics Research Association (Great Britain) polystyrene sample: From
light scattering data in benzene and 2-butanone at 30°C measured by H. S. * * National Bureau of Standards (USA) broad MWD standard polystyrene: MW data are
few broad MWD polystyrenes. Apparently these samples are eluted at a critical region near the aL limit, i.e., about 28 ml elution volume region, where, the MW
calibration is highly distorted, a is sensitive to v, and therefore the correction factors vary rapidly with v. Nevertheless, the corrections based on the present scheme appears to be satisfactory or at least leaving only a tolerable discrepancy between
the corrected and supposed-to-be true values. A few other remarks should be added here on the use of a high-speed GPC unit:
They are the problems of flow-rate and sample-size dependences of chromatogram shape. In Table I we have seen that the peak elution volume ve shifts to a larger v
value as flow-rate increases. A higher speed run results in not only the shift of ve but a more significant broadening and tailing (to larger v side). This problem may
be avoided operationally by setting up the MW and a calibrations for each series or runs of different flow-rate. In fact the procedures mentioned above were applied
T. KOTAKA, H. Suzuki, and H. INAGAKI
to the 1 ml/min and 2 ml/min runs as well. And we found satisfactory results. However the second problem, i.e., the sample-size dependence appears to be more
problematic. Presumably because of the small total volume of a high-speed GPC, overloading effects easily become apparent: Chromatogram shape is quite sensitive to the injection volume, and is somewhat less but still significantly sensitive to the concentration of stock solutions (especially when they are high, say, >0.5%).14) Usually a larger sample size results in shifting of chromatogram to larger v side and more serious tailing. In the above analysis, we have set up a standard working condition for both standard and test samples, and handled their chromatograms as they were. Obviously it is desirable to establish a method of eliminating such a sample-size dependence before applying the calibration procedures such as proposed
here. In our preliminary trial we observed that the v, shifts to lower v side more significantly for high MW standards as the sample-size is decreased: The vL limit. shifts to lower v side, and the MW calibration becomes closer to a logarithmic straight line.14,15) Therefore the decrease in sample-size creates a favorable condition to carry out a quantitative analysis, except that it reduces the detector response which is of course proportional to the sample size. This is particularly important in dealing with broad MWD samples which spread out in the entire v region. An extensive study on this problem is now in progress. The results will be published elsewhere shortly.
The computer work was performed with a Facom 230-48 digital computer
(Fujitsu Ltd., Tokyo) of Computer Laboratory of this Institute. We thank the staffs of the Laboratory, especially Dr. K. Kajiwara for valuable advices on the computer handling. This work was a part of the presentation given by TK at 1975 GPC seminar held at Pittsburgh, PA., during October 15 to 17, 1975.
(1) J. C. Moore, J. Polym. Sci., A2, 835 (1964). (2) W. Heitz and S. Potnis, Makromol. Chem., 145, 141 (1971). (3) R. J. Limpert, R. L. Cotter, and W. A. Dark, Waters Tech. Report No. 919 (1974). (4) Y. Kato, S. Kido, M. Yamamoto, and T. Hashimoto, J. Polym. Sci. (Physics), 12, 1339
(1974). (5) A. C. Ouano, W. Kaye, J. Polym. Sci. (Chemistry), 12, 1151 (1974). (6) A. C. Ouano, J. Polym. Sci., in press. (7) L. H. Tung, J. Appl. Polym. Sci., 10, 375, 1271 (1966). (8) L. H. Tung, ibid., 10, 1261 (1966). (9) H. E. Pickett, M. J. R. Cantow, and J. F. Hohnson, J. Polym. Sci., C21, 47 (1968).
(10) T. Kotaka, J. Appl. Polym. Sci., in press. (11) T. Kotaka, Angew. Makromol. Chem., to be published.
(12) See for example; (a) G. Meyerhoff, J. Polym. Sci., C21, 31 (1968); (b) J. H. Hazel, L. A. Prince, and H. E. Stapelfeldt, ibid., C21, 43 (1968).
(13) See for example: (a) M. Hess, R. F. Kratz, J. Polym. Sci. A2, 4, 731 (1966); (b) W. N. Smith, J. Appi. Polym. Sci., 11, 639 (1967); (c) T. H. Duerksen and A. E. Hamielec, J.
Polym. Sci., C21, 83 (1968) ; (d) L. H. Tung, J. Appi. Polym. Sci., 13, 775 (1969) ; (e) S. T.
High Speed GPC
Balke and A. E. Hamielec, ibid., 13, 1381 (1969) ; (f) K. S. Chang and R. Y. H. Huang, ibid., 13, 1459 (1969); (g) A. E. Hamielec, ibid., 14, 1519 (1970); (h) T. Ishige, S. I.
Lee and A. E. Hamielec, ibid., 15, 1607 (1971).
(14) H. Suzuki and T. Kotaka, Unpublished experiments, 1975-1976. (15) S, Mori, personal communication, 1975.